Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- Viscoelastic Damping: Classical Models by Mohammad Tawfik 3641 views
- Modeling viscoelastic-damping-for-d... by Can Ozcan 1534 views
- Viscoelastic Damping: Zener model by Mohammad Tawfik 4998 views
- Rheology by Prof. Dr. Basavar... 8182 views
- Rheology by Rajveer Bhaskar 12171 views
- Toward overcoming the concept of ef... by Alessandro Palmeri 4433 views

No Downloads

Total views

504

On SlideShare

0

From Embeds

0

Number of Embeds

3

Shares

0

Downloads

10

Comments

0

Likes

1

No embeds

No notes for slide

- 1. Oversimpliﬁed Viscoelasticity THE MAXWELL MODEL At time t = 0, suddenly deform to constant displacement Xo. The force F is the same in the spring and the dashpot. F = KeXe = Kv(dXv/dt) (1-20) Xe is the displacement of the spring Xv is the displacement of the dashpot Ke is the linear spring constant (ratio of force and displacement, units N/m) Kv is the linear dashpot constant (ratio of force and velocity, units Ns/m) The total displacement Xo is the sum of the two displacements (Xo is independent of time) Xo = Xe + Xv (1-21) 1
- 2. Oversimpliﬁed Viscoelasticity THE MAXWELL MODEL (p. 2) Thus: Ke(Xo − Xv) = Kv(dXv/dt) with B. C. Xv = 0 at t = 0 (1-22) (Ke/Kv)dt = dXv/(Xo − Xv) Integrate: (Ke/Kv)t = − ln(Xo − Xv) + C Apply B. C.: Xv = 0 at t = 0 means C = ln(Xo) −(Ke/Kv)t = ln[(Xo − Xv)/Xo] (Xo − Xv)/Xo = exp(−Ket/Kv) Thus: F(t) = KeXo exp(−Ket/Kv) (1-23) The force from our constant stretch experiment decays exponentially with time in the Maxwell Model. The relaxation time is λ ≡ Kv/Ke (units s) The force drops to 1/e of its initial value at the relaxation time λ. Initially the force is F(0) = KeXo, the force in the spring, but eventually the force decays to zero F(∞) = 0. 2
- 3. Oversimpliﬁed Viscoelasticity THE MAXWELL MODEL (p. 3) Constant Area A means stress σ(t) = F(t)/A σ(0) ≡ σ0 = KeXo/A Maxwell Model Stress Relaxation: σ(t) = σ0 exp(−t/λ) Figure 1: Stress Relaxation of a Maxwell Element 3
- 4. Oversimpliﬁed Viscoelasticity THE MAXWELL MODEL (p. 4) A creep experiment applies constant force F (or constant stress). F = KeXe = Kv(dXv/dt) (1-20) Thus: Xe = F/Ke and dXv/dt = F/Kv with B. C. Xv = 0 at t = 0 Integrate: Xv = Ft/Kv The total displacement is Xo = Xe + Xv = F(1/Ke + t/Kv) Strain γ ≡ Xo/L0 γ = (1 + Ket/Kv)F/(KeL0) The instantaneous strain in the spring is γ0 ≡ F/(KeL0) and the relax- ation time is again λ ≡ Kv/Ke. Maxwell Model Creep: γ(t) = γ0(1 + t/λ) Figure 2: Creep of a Maxwell Element 4
- 5. Oversimpliﬁed Viscoelasticity THE VOIGT MODEL Figure 3: Voigt Element: A Spring and a Dashpot in Parallel At time t = 0, apply a constant force F. The displacement X is the same in the spring and the dashpot. The force F is the sum of forces in the spring and the dashpot. F = KeX + Kv(dX/dt) with B. C. X = 0 at t = 0 (1-18) (Ke/Kv)dt = dX/[(F/Ke) − X] Integrate: (Ke/Kv)t = − ln[(F/Ke) − X] + C Apply B. C.: X = 0 at t = 0 means C = ln(F/Ke) −(Ke/Kv)t = ln[1 − XKe/F] 1 − XKe/F = exp(−Ket/Kv) Thus: X(t) = (F/Ke)[1 − exp(−Ket/Kv)] (1-19) 5
- 6. Oversimpliﬁed Viscoelasticity THE VOIGT MODEL (p. 2) X(t) = (F/Ke)[1 − exp(−Ket/Kv)] (1-19) We again have strain γ(t) ≡ X(t)/L0, and relaxation time λ ≡ Kv/Ke. We deﬁne γ∞ ≡ F/(KeL0) as the long time limit of the strain. Voigt Model Creep: γ(t) = γ∞[1 − exp(−t/λ)] Figure 4: Creep of a Voigt Element The Voigt Model captures the essential physics of creep for a viscoelastic solid. 6
- 7. Oversimpliﬁed Viscoelasticity MAXWELL AND VOIGT MODELS IN SERIES Strains of elements combined in series always add in creep. γ(t) = γMaxwell(t) + γV oigt(t) γ(t) = γ0(1 + t/λ) + γ∞[1 − exp(−t/λ)] Figure 5: Maxwell and Voigt Elements in Series and their Strain in Creep Maxwell and Voigt Elements in Series capture the essential physics of creep for a viscoelastic liquid. 7
- 8. Rheological Terminology THE JARGON OF STRANGE FLUIDS Dilatancy n. Increase in apparent viscosity with shear rate (also shear- thickening). Rare, but seen in some solutions of associating polymers. Rheopexy n. Apparent viscosity increases with time at a given rate (also anti-thixotropy or structure-building). Rare, but seen in some suspensions. Thixotropy n. Apparent viscosity decreases with time at a given rate (also structure-breaking). Common for concentrated suspensions. Figure 6: Thixotropic behavior of a structured ﬂuid. Shear-thinning n. Decrease in apparent viscosity with shear rate. Very important for nearly all polymers and suspensions. Yield Stress n. The stress required for a structured ﬂuid to ﬂow (also Bingham stress). Common for concentrated suspensions and liquid crys- tals. 8
- 9. Yield Stress THE BINGHAM MODEL Structured ﬂuids, such as concentrated suspensions and liquid crystals show solid rheological response at low stress levels. The simplest model for this class of ﬂow is the Bingham Model. σ = Gγ σ < σ0 σ0 + ηp ˙γ σ > σ0 (1-24) σ0 is the yield stress, below which there is no ﬂow, and above which ﬂow occurs with σ0 of the stress being used to maintain the liquid response, and the remainder (ηp ˙γ) causing simple Newtonian ﬂow. Figure 7: Flow Curve of a Bingham Plastic compared to Newtonian and shear-thinning ﬂuids. Flexible polymer melts and solutions are either Newtonian (σ = η ˙γ) or shear-thinning (meaning that the apparent viscosity decreases with shear rate) but do NOT have a yield stress. 9
- 10. Origins of Elasticity in Polymer Liquids The conﬁguration of a polymer chain in a melt is a random walk because it maximizes conﬁgurational entropy. Flow Field =⇒ Stretch Chain =⇒ Lower Entropy Conﬁguration Figure 8: By stretching the chain, the number of conﬁgurations is reduced, which decreases the entropy (and requires work). Using Statistical Mechanics, it is easy to show that the chain actually behaves like a linear spring. The (entropic) free energy G is quadratic in the end-to-end distance R. G = 3kTR2 2Nb2 k is Boltzmann’s constant T is absolute temperature N is the number of monomers in the chain b is the monomer size In the upstretched state R2 = Nb2 , and the conﬁgurational free energy is 3kT/2. The force required to stretch the chain is F = ∂G ∂R = 3kTR Nb2 This is precisely why a rubber band behaves like a linear spring. 10

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment